Research Article  Open Access
Partha Sona Maji, Partha Roy Chaudhuri, "A New Design for AllNormal Near Zero Dispersion Photonic Crystal Fiber with Selective Liquid Infiltration for Broadband Supercontinuum Generation at 1.55 μm", Journal of Photonics, vol. 2014, Article ID 728592, 9 pages, 2014. https://doi.org/10.1155/2014/728592
A New Design for AllNormal Near Zero Dispersion Photonic Crystal Fiber with Selective Liquid Infiltration for Broadband Supercontinuum Generation at 1.55 μm
Abstract
A new design of allnormal and near zero flattened dispersion based on allsilica photonic crystal fibers (PCFs) using selectively liquid infiltration technique has been proposed to realize smooth broadband supercontinuum generation (SCG). The investigation gives the details of the effect of different geometrical parameters along with the infiltrating liquids on the dispersion characteristics of the fiber. Numerical investigations establish a dispersion value of −0.48 ps/nm/km around the wavelength of 1.55 μm. The optimized design has been found to be suitable for SCG around the C band of wavelength with flat broadband wavelength band (375 nm bandwidth) and smooth spectrum with only a meter long of the PCF. The proposed structure also demonstrates good tunable properties that can help correct possible fabrication mismatch towards a better optimization design for various optical communication systems.
1. Introduction
Broadband smooth flattened supercontinuum generation (SCG) has been the target for the researchers for its enormous applications in the field of metrology, optical sensing, optical coherence tomography, wavelength conversion, and so forth [1]. Recent developments for midinfrared (MIR) SC source have been investigated based on nonsilica fibers [2, 3]. Unconventional PCFs based on aperiodic structure have also been investigated [4]. However, achieving flat broadband smooth SC sources for IR applications remains challenging [1]. One of the foremost requirements of generating broadband flattened SCG is to achieve near zero flattened dispersion around a targeted wavelength. Photonic crystal fibers (PCFs) [5, 6], which enjoys some unique properties like wide band single mode operation, great controllability over dispersion properties, and higher nonlinearity, has been the target host for SCG for the last decades [1]. Researchers have worked on designing novel dispersion profiles with variable airhole diameter in the cladding [7–13] and this design can be further manipulated for SC generation by pumping at the near zero wavelength [9, 14]. However, the realizing technology of complicated structures or PCF having airholes of different diameters in microstructure cladding remains truly challenging. An alternative route of achieving similar performance is shown to be practicable by filling the airholes with liquid crystals [15, 16] or by various liquids such as polymers [17], water [18], and ethanol [19]. Tunable photonic band gap (PBG) effect and longperiod fiber grating have been successfully realized with liquidfilled PCFs [20]. Theoretical design of dispersion management by filling the airholes of the PCF with selective liquids for both single wavelength and broadband wavelength applications has been studied [21, 22]. In the present work, a new design of silica based PCF with allnormal near zero chromatic dispersion around the desired wavelength of 1.55 μm through selectively liquidfilled inner airholes has been proposed and the optimized design has been targeted for achieving smooth and flattened broadband SC spectra. As most of the power resides within the core of the PCF, liquid infiltration in airholes will have the only effect in dispersion controllability. We also investigate the temperature dependence of the liquidfilled PCFs for better optimization design with its tunable property of shifting dispersion peak for optical communication systems. The main advantage with this approach is that we need not require different airholes in the cladding to realize near zero dispersion at the desired wavelength; also we can tune the dispersion towards a better optimized design by changing the temperature of the liquid and thereby achieving highly smooth and flat broadband SC spectra with only a meter long of the fiber.
2. LiquidFilled Photonic Crystal Fiber and Related Issues
Conventional PCFs have cladding structures formed by airholes with the same diameter arranged in a regular triangular or square lattice. By altering the PCF geometrical parameters, namely, holetohole spacing () and airhole diameter (), the modal properties, in particular, the dispersion properties can be easily engineered [5, 6]. However, the dispersion slope of such PCFs having airholes of the same diameter cannot be tailored in a wide wavelength range. The current research aims to achieve allnormal dispersion close to zero at a desired wavelength with a flat slope of the dispersion curve using regular triangularlattice structure having airholes of the same size uniformly distributed in the cladding. A common route to realize these goals of flat dispersion around a specific wavelength is by varying the size of airholes in different layers and is well known in [7–12]. Because of the fabrication limitation, the concept finds limited use as a practical fiber. This research looks for the achievement of these targets through a regular conventional PCF by incorporating the effects of filling airhole ring with a liquid of predetermined refractive index (RI). Depending upon the refractive indices of the infiltrating liquid to the airholes, the local refractive indices of the layer can be modified. In that way, the effect of variable airhole diameter can be realized by infiltrating the airholes with liquids of different refractive indices. Depending upon the RI of the infiltrating liquid, we could have the effect of different airhole diameter.
The fabrication of such a fiber is simplified due to the uniformity of the airholes in the cladding. To manufacture these PCFs, one must first selectively block specified airholes and infuse the liquid into the unblocked holes. One possible way is to employ the fusion splicing technique [18–20]. The inner ring of the airholes can be infiltrated with liquid, first by fusing the outer rings of airholes with tailored electric arc energies and fusion times [23] and then by immersing one end of the fiber in a liquid reservoir and applying vacuum to the other end of the fiber [18]. This can be a possible way to infiltrate liquid in our case. Another way of selective plug specified airhole layers in the PCFs is to use microscopically positioning tips with glue [24]. Not only airhole layers but also a single airhole can be easily blocked by using this technique. In spite of the above methods, one can also selectively infiltrate the liquid into specified airhole layers from a macroscopic fiber preform to a connected microstructured PCF by using an applied pressure [21]. With the optimized airhole diameters of the order of 0.60 μm, it should be easy to collapse the airholes and fill the liquid into the airholes with such dimensions. It is also interesting to note that PCFs with similar or smaller airhole diameter was realized [25], making the proposed design practically achievable. With the advancement of technology, a good precision of the PCF parameters can be easily implemented.
There are certain issues related to the infiltration of liquid to the airholes, such as whether the fluid wets glass and how viscous it is. If the liquid does not wet glass, then surface tension will oppose entry of the liquid into the airhole, thereby making the process difficult to realize. The required pressure to push such a liquid into the airholes can be worked out with the value of its surface tension and contact angle. With an airhole diameter of the order of 0.60 μm, pressure by a vacuum pump will be sufficient.
If the fluid does wet glass, then the airhole should be filled but the fillingup speed will depend upon viscosity. It can be worked out how quickly the airholes will be filled using the expressions for Poiseuille flow in a pipe [26]. In other words, the airholes can be filled (and how quickly), with the given values for surface tension, contact angle, and viscosity. With the fast advancement of the technology, submicron filling of airholes will not be very difficult to achieve.
The selective hole filling technique provides a couple of advantages. Firstly, all the airholes are of the same diameter, which is easier to be fabricated compared to fibers with multiple different submicron airhole sizes. Secondly, a regular PCF with selective infiltration with a liquid provides huge flexibility for tremendous applications. This is why the paper pursues selective airhole filling approach towards the target of allnormal near zero dispersion in a microstructured optical fiber. Notably, the technique comes out in designing fibers for various other applications [21, 22, 27–32].
3. Analysis Method and Design Optimization of the PCF
As an initial attempt, we consider a regular PCF with four rings of airholes with symmetry with the central airhole missing like normal indexguiding PCF as shown in Figure 1. The inner ring of airholes is infiltrated with a liquid of certain RI’s. Throughout our design study we have kept higher airfiling fraction, thereby reducing the confinement loss of the structure. As can be seen from our numerical results, we need only a meter long of such a fiber; the propagation loss of the high power spectrum can therefore be highly reduced. By optimizing the RI value () of the infiltrating liquid combined with PCF geometrical parameters, namely, pitch () and airhole diameter (), allnormal near zero dispersion around a particular wavelength can be realized.
3.1. Dispersion Analysis
Modal fields as well as dispersion parameters are calculated by using commercially available CUDOS software along with MATLAB for numerically calculating the dispersion relation. The total dispersion () is computed with [33]:
Here stands for the real part of the effective indices, is the speed of light in vacuum, and is the wavelength.
3.2. Supercontinuum Generation (SCG) Analysis
The SCG with the liquid filled near zero allnormal dispersion silica based PCF for smooth flattened broadband spectra has been studied by solving the nonlinear Schrödinger equation (NLSE) [33] describing the pulse propagation through the fiber length. The NLSE takes into account the contributions of the linear effects (attenuation, chromatic dispersion, and highorder dispersions) and the nonlinear effects (selfphase modulation, stimulated Raman scattering, and selfsteepening). NLSE for slowly varying pulse envelope in the retarded time frame is given through (2) as follows: where is the loss coefficient, are the th order dispersion, is the input pulse frequency, is the present time frame, and is the fractional contribution due to delayed Raman function [33, 34]. The nonlinear coefficient is given by (3) as follows: where is the nonlinear refractive indices of silica and is the effective area at the pumping wavelength .
3.3. Optimization for AllNormal Near Zero Dispersion at the Target Wavelength
The nonlinear effects in a PCF strongly depend on the dispersive characteristic and the length of the employed optical fiber [1]. In particular, with reference to SCG, the shape of the total dispersion curve can be tailored to obtain a broadband output spectrum. The approach of the present research of optimization towards designing near zero allnormal flat dispersion relies on varying multidimensional parameter space that consists of the liquid RI (), the pitch , and airhole diameter (). The procedure is followed in three steps. In the first step, the sensitivity of the variation of the parameters towards the total dispersion has been illustrated by varying one of the design parameters on the dispersion keeping other parameters constant. In the second stage, we took one of the parameters fixed (value obtained from the first step) and optimized the other parameters towards the target. Once one parameter is optimized, we reoptimize the design by adjusting other parameters. In the third stage we select a practical liquid (wavelength dependent RI) close to the optimized RI and optimize the other parameters to achieve the target of allnormal near zero dispersion. The first stage of the design optimization is presented as follows. Figure 2 shows the effect of on the values. For a particular , the value of initially increases to reach a maximum and then starts decreasing. The graph clearly indicates that with an increase of , the maximum of is redshifted and the dispersion becomes more flatter with wavelengths, while for smaller wavelengths they are almost parallel without much change in the slope. The flatness can be understood from the following analogy: the dispersion value from the peak reduces by an amount of 25 ps/nm/km for a wavelength range of 794 nm for = 1.00 μm, while for the same values of dispersion range, the wavelength range comes out to be 760 nm for μm. This can be attributed to the fact that, for higher , material dispersion dominates, reducing the effect of waveguide dispersion. From Figure 3 it can be observed that both the magnitude and the slope of are affected for different values of . An increase of causes a blueshift of the dispersion peak and the dispersion values also increase. The effect of varying the airhole diameter without changing the other parameters is depicted in Figure 4. It should be noted that we have changed the diameter of all the airholes including those containing the infiltrating liquid. An interesting observation can be found out that, with an increase of , the dispersion seems to be converging for higher wavelengths while the peak again gets redshifted but with a steeper slope than that of Figure 2. The convergence can be attributed to the increased effect of waveguide dispersion to the total dispersion. Thus, the effect of varying the influences the total dispersion, whereas has the desired effect of modifying the dispersion slope, and varying modifies both the slope and dispersion.
Then, we started the second stage of the optimization procedure as the following. For this step we tried to keep nearer to 1.0 μm such that we could have smaller effective area which in turn will enhance nonlinearity. Starting with and , the values of the are changed progressively to get a near zero profile of the dispersion. To have higher values of nonlinear coefficient, we kept the values around 0.90 μm. Then the values of airhole diameter and are changed progressively to either raise or lower the dispersion and change the slope. During the process we tried to keep the values of the parameters such that the values of the parameters remain practically feasible. Following the above steps, we have obtained an allnormal near zero dispersion in the wavelength around 1570 nm with value of −0.41 ps/nm/km with μm and μm and as demonstrated in Figure 5.
Having obtained a preliminary design using an artificial, dispersionless liquid, we continue with the third optimization stage. We select oil (calling it as oil number 1) whose RI is close to the above optimized value in the target communication wavelength band and is given by Cauchy (4) (available with M/S Cargile lab., USA [35]).
Cauchy equation for oil number 1 is known to be [35] where are in Angstrom.
With this liquid an allnormal near zero dispersion PCF with value of −0.48 ps/(nm.km) around 1550 nm of wavelength has been achieved with the designing PCF parameters of μm with μm as shown in Figure 6. Now as we see the value is higher than the accepted value for endlessly “singlemode” operation. To achieve our target, we needed to make a tradeoff between a pure singlemode guiding and few higher order mode guiding. Our numerical study reveals that with our present optimize value the next higher order mode can coexist with the fundamental one; however the confinement loss of the mode is found out to be about hundred times of magnitude higher than that of the fundamental mode throughout the spectral range considered (specially at the pumping wavelength) and hence would leak away with propagation within a very short length of the designed fiber. This would make the designed fiber an “effectively singlemode fiber.” The effect of liquid infiltration upon dispersion has been presented in Figure 7. The figure clearly reveals the determining effect of the liquid infiltration in the airholes as not only a drastic change but also a slope reversal of the dispersion could be observed. Total dispersion along with the contribution of the material dispersion of the liquid and background silica material towards the total dispersion has been shown in Figure 8 for the above optimized structure. The new control technique applied to the design of PCFs with desired dispersion properties can be widely used for specific applications such us control of SCG, sensors, and broadband transmission [1].
4. Numerical Analysis for SCG with the Optimized Near Zero AllNormal Dispersion PCF
NLSE, as mentioned in (2), is solved numerically by using the split step Fourier transform based beam propagation code developed by COSTP11 [36]. In our study, we have considered the pumping of laser power pulses with hyperbolic secant field profile emerging from a laser with full width at half maximum (FWHM) of 1.5 ps. In our calculations we set the pump wavelength of μm, the closest to zero in the normal dispersion regime, in order to generate the broadest spectra. Consequently, the spectral widening is dominated by selfphase modulation (SPM) followed by optical wave breaking and the noisesensitive soliton dynamics are suppressed by pumping in the normal dispersion region in such fibers. The soliton effect, for example, soliton fission, is completely removed, giving rise to the smooth spectra. Optimization of the allnormal dispersion fiber design allowed us to generate ultrabroadband, flat top, and smooth SC generation. An effective area of 4.03 μm^{2} and nonlinear coefficient W^{−1}·km^{−1} are achieved in the optimized PCF with μm and μm at the pumping wavelength. The input pulse power has been kept to be 4.0 kW with FWHM of 1.5 ps. A possible source for such a pump can be the commercially available Er3+, Yb3+ doped silicate based fiber laser emitting around 1550 nm of wavelength [37]. The calculated values of higher order betas are presented in Table 1. The spectrum evolution of the fiber after it evolves through each 25 cm of the fiber with the above parameters has been shown in Figure 9. The spectrum spreads for a wide wavelength range, ranging from 1300 nm to 1750 nm. The intensity is calculated using the usual notation with Intensity . It can be observed that as the pulse propagates through the fiber the peak power reduces, creating new peaks on both sides of the input pulse almost symmetrically. The evolution of the spectrum as a function of propagation distance has been shown in Figure 10 which clearly shows the spreading of the pulse taking almost symmetrically around the pumping wavelength. The graph clearly indicates that after travelling a distance of 1.2 meters, the broadband spectrum spread for a wide wavelength range from 1300 nm to 1750 nm. One of the most notable features of the SC spectrum is the spectral broadening which is accompanied with an oscillating nature covering the whole spectrum. The spectrum consists of many small peaks. This particular nature is a typical pattern due to selfphase modulation (SPM), which is assumed to be dominating nonlinear effect for the spectral broadening. The multipeak structure in the system is the result of interference between the same optical frequencies in the pulse and the relatively smoother SC generation results from the combination effect of SPM and allnormal near zero flat dispersion nature of the fiber. We have calculated the spectral width of the broadband flat SC spectrum according to Begum et al. [14], where they have calculated the FWHM at the negative value of the intensity points corresponding to the peak maximum value. With the same analogy, numerical calculations show a bandwidth of 375 nm with our optimized fiber. However with another way, the intensity bandwidth can be calculated at −20 dB from the peak point. The numerical calculation shows a 20 dB bandwidth of spectral width of 285 nm that can be achieved with a fiber length of 1.2 meter as shown in Figure 11.

5. Tunable Properties of Inner Ring LiquidFilled PCFs
It is well known that the dispersion can be tailored in a PCF according to the requirement by changing the geometrical parameters. However, once a design is fixed and fabricated the dispersion of that particular fiber is also fixed. So, to have a different or optimized design we need another fiber to be fabricated. Now here comes the advantage of liquidfilled PCF. Fluidfilled PCFs have created novel opportunities for tunable dispersion control, with applications in tunable delay lines, nonlinear optics, and long period grating designs [38]. Here in this type of selective liquid infiltrated PCF, we can change the RI of the infiltrating liquid by changing the temperature of the infiltrating liquid and can tune the dispersion properties according to the requirement. As the temperature coefficient of the liquids available with M/s Cargile lab [35] is of the order of °C which is much larger than that of fused silica, the smaller changes of temperature will affect the RI of the liquid only. We have considered the optimized design shown in Figure 6 and we demonstrate the tunability property of the liquid by changing the temperature of the liquid. Figure 12 shows the dispersion characteristics for five different temperature of the liquid. It can be seen from the figure that with the increase of the temperature the peak value of the dispersion shifts away from the zero dispersion value. The peak dispersion and the corresponding variation of the peak dispersion wavelength for different temperature are demonstrated in Figure 13. The peak dispersion value with temperature shows a linear relationship with a negative slope of −0.31084 ps/nm/km/°C. Wavelength corresponding to peak dispersion for different temperature has been presented in Figure 13(b). The graph presents a linear relationship between the corresponding wavelength with temperature with a positive slope of 0.65 nm/°C. So we can tune the temperature of the liquid according to the requirement to obtain an optimized/required design. Our numerical calculations demonstrate that around the temperature of 23.5°C, we could achieve an allnormal flat dispersion PCF with a peak value of −0.089 ps/nm/km around 1550 nm of wavelength. This design will be more demanding for the current target of allnormal flat dispersion around 1550 nm. So with the tunability property of the infiltrating liquid we can easily tune the peak dispersion just by changing the temperature of the liquid for a fabricated PCF.
(a)
(b)
6. Conclusion
We have demonstrated a new design of allnormal near zero dispersion PCF based on selectively liquid infiltration and explored its properties for flattened broadband SC generation in near IR wavelength regions. We have studied the effect of individual PCF parameters, namely, Λ and , along with infiltrating liquid () towards the target of allnormal near zero dispersion PCF around the communication wavelength window. Our study reveals that varying influences the total dispersion, whereas has the desired effect of modifying the dispersion slope and varying modifies both the slope and the dispersion. Based on the above findings, we have achieved an allnormal near zero dispersion PCF with value of −0.48 ps/(nm·km) around 1550 nm of wavelength with the designing PCF parameters of μm with μm and oil number 1. Our study reveals that by adjusting the different parameters, near ZDW can be tuned according to the requirement. With the above designed PCF, we have obtained a smooth and broadband spectra ranging from 1350 nm to 1725 nm, that is, for a bandwidth of 375 nm with 1.2 meter length of the fiber. We have also demonstrated the tunability properties of the optimized PCF. The peak wavelength corresponding to allnormal flat dispersion can be well tuned by the refractive index of the liquid which can be controlled by the operation temperature. By changing the operational temperature to 23.5°C we could achieve a peak dispersion of −0.089 ps/nm/km around 1550 nm of wavelength with our optimized design. The tunability of the liquidfilled PCF can be utilized for wide wavelength range applications and also to correct possible fabrication mismatches in the geometry of PCF structures. The significance of this work is that it provides a new type of dispersion engineered silica based PCF for near Infrared (IR) SC source with flat broadband spectrum with about a meter long of the fiber which can be useful for applications in metrology, spectroscopy, and optical coherence tomography in the near infrared region.
Conflict of Interests
The authors declare that there is no conflict of interests regarding the publication of this paper.
Acknowledgments
The authors would like to thank Dr. Boris Kuhlmey, University of Sydney, Australia, for providing valuable suggestions in understanding the software for designing and studying the properties of different structures. Thanks are also due to Dr. Alessandro Tonello of Xlim Institute, UMR CNRS Limoges Cedex, France, for providing valuable suggestion in developing and understanding the NLSE codes. The authors acknowledge sincerely the Defence Research and Development Organization, Govt. of India and CRF of IIT Kharagpur for the financial support to carry out this research.
References
 J. M. Dudley, G. Genty, and S. Coen, “Supercontinuum generation in photonic crystal fiber,” Reviews of Modern Physics, vol. 78, no. 4, pp. 135–184, 2006. View at: Publisher Site  Google Scholar
 J. Swiderski, F. Théberge, M. Michalska, P. Mathieu, and D. Vincent, “High average power supercontinuum generation in a fluoroindate fiber,” Laser Physics Letters, vol. 11, pp. 015106–015109, 2014. View at: Google Scholar
 G. Sobon, M. Klimczak, J. Sotor et al., “Infrared supercontinuum generation in softglass photonic crystal fibers pumped at 1560 nm,” Optical Materials Express, vol. 4, pp. 7–15, 2014. View at: Google Scholar
 A. di Tommaso, M. de Sario, L. Mescia, and F. Prudenzano, “Numerical analysis of aperiodic photonic crystal fiber structures for supercontinuum generation,” Optical Engineering, vol. 51, pp. 0350031–0350037, 2012. View at: Google Scholar
 J. Broeng, D. Mogilevstev, S. E. Barkou, and A. Bjarklev, “Photonic crystal fibers: a new class of optical waveguides,” Optical Fiber Technology, vol. 5, no. 3, pp. 305–330, 1999. View at: Publisher Site  Google Scholar
 P. S. J. Russell, “Photoniccrystal fibers,” Journal of Lightwave Technology, vol. 24, no. 12, pp. 4729–4749, 2006. View at: Publisher Site  Google Scholar
 K. Saitoh, N. J. Florous, and M. Koshiba, “Theoretical realization of holey fiber with flat chromatic dispersion and large mode area: an intriguing defected approach,” Optics Letters, vol. 31, no. 1, pp. 26–28, 2006. View at: Publisher Site  Google Scholar
 N. Florous, K. Saitoh, and M. Koshiba, “The role of artificial defects for engineering large effective mode area, flat chromatic dispersion, and low leakage losses in photonic crystal fibers: towards high speed reconfigurable transmission platforms,” Optics Express, vol. 14, no. 2, pp. 901–913, 2006. View at: Publisher Site  Google Scholar
 K. Saitoh and M. Koshiba, “Highly nonlinear dispersionflattened photonic crystal fibers for supercontinuum generation in a telecommunication window,” Optics Express, vol. 12, no. 10, pp. 2027–2032, 2004. View at: Publisher Site  Google Scholar
 K. Saitoh, M. Koshiba, T. Hasegawa, and E. Sasaoka, “Chromatic dispersion control in photonic crystal fibers: application to ultraflattened dispersion,” Optics Express, vol. 11, no. 8, pp. 843–852, 2003. View at: Google Scholar
 F. Poletti, V. Finazzi, T. M. Monro, N. G. R. Broderick, V. Tse, and D. J. Richardson, “Inverse design and fabrication tolerances of ultraflattened dispersion holey fibers,” Optics Express, vol. 13, no. 10, pp. 3728–3736, 2005. View at: Publisher Site  Google Scholar
 T.L. Wu and C.H. Chao, “A novel ultraflattened dispersion photonic crystal fiber,” IEEE Photonics Technology Letters, vol. 17, no. 1, pp. 67–69, 2005. View at: Publisher Site  Google Scholar
 X. Zhao, G. Zhou, L. Shuguang et al., “Photonic crystal fiber for dispersion compensation,” Applied Optics, vol. 47, no. 28, pp. 5190–5196, 2008. View at: Publisher Site  Google Scholar
 F. Begum, Y. Namihira, T. Kinjo, and S. Kaijage, “Supercontinuum generation in square photonic crystal fiber with nearly zero ultraflattened chromatic dispersion and fabrication tolerance analysis,” Optics Communications, vol. 284, no. 4, pp. 965–970, 2011. View at: Publisher Site  Google Scholar
 C. Zhang, G. Kai, Z. Wang et al., “Transformation of a transmission mechanism by filling the holes of normal silicaguiding microstructure fibers with nematic liquid crystal,” Optics Letters, vol. 30, no. 18, pp. 2372–2374, 2005. View at: Publisher Site  Google Scholar
 T. T. Alkeskjold, J. Lægsgaard, A. Bjarklev et al., “Highly tunable largecore singlemode liquidcrystal photonic bandgap fiber,” Applied Optics, vol. 45, no. 10, pp. 2261–2264, 2006. View at: Publisher Site  Google Scholar
 B. J. Eggleton, C. Kerbage, P. S. Westbrook, R. S. Windeler, and A. Hale, “Microstructured optical fiber devices,” Optics Express, vol. 9, no. 13, pp. 698–713, 2001. View at: Google Scholar
 C. Martelli, J. Canning, K. Lyytikainen, and N. Groothoff, “Watercore fresnel fiber,” Optics Express, vol. 13, no. 10, pp. 3890–3895, 2005. View at: Publisher Site  Google Scholar
 S. Yiou, P. Delaye, A. Rouvie et al., “Stimulated Raman scattering in an ethanol core microstructured optical fiber,” Optics Express, vol. 13, no. 12, pp. 4786–4791, 2005. View at: Publisher Site  Google Scholar
 C.P. Yu and J.H. Liou, “Selectively liquidfilled photonic crystal fibers for optical devices,” Optics Express, vol. 17, no. 11, pp. 8729–8734, 2009. View at: Publisher Site  Google Scholar
 K. M. Gundu, M. Kolesik, J. V. Moloney, and K. S. Lee, “Ultraflatteneddispersion selectively liquidfilled photonic crystal fibers,” Optics Express, vol. 14, no. 15, pp. 6870–6878, 2006. View at: Publisher Site  Google Scholar
 C. P. Yu, J. H. Liou, S. S. Huang, and H. C. Chang, “Tunable dualcore liquidfilled photonic crystal fibers for dispersion compensation,” Optics Express, vol. 16, no. 7, pp. 4443–4451, 2008. View at: Publisher Site  Google Scholar
 L. Xiao, W. Jin, M. S. Demokan, H. L. Ho, Y. L. Hoo, and C. Zhao, “Fabrication of selective injection microstructured optical fibers with a conventional fusion splicer,” Optics Express, vol. 13, no. 22, pp. 9014–9022, 2005. View at: Publisher Site  Google Scholar
 A. Witkowska, K. Lai, S. G. LeonSaval, W. J. Wadsworth, and T. A. Birks, “Allfiber anamorphic coreshape transitions,” Optics Letters, vol. 31, no. 18, pp. 2672–2674, 2006. View at: Publisher Site  Google Scholar
 W. H. Reeves, J. C. Knight, P. S. J. Russell, and P. J. Roberts, “Demonstration of ultraflattened dispersion in photonic crystal fibers,” Optics Express, vol. 10, no. 14, pp. 609–613, 2002. View at: Google Scholar
 E. W. Washburn, “The dynamics of capillary flow,” Physical Review, vol. 17, pp. 273–283, 1921. View at: Publisher Site  Google Scholar
 J. H. Liou, S. S. Huang, and C. P. Yu, “Lossreduced highly birefringent selectively liquidfilled photonic crystal fibers,” Optics Communications, vol. 283, no. 6, pp. 971–974, 2010. View at: Publisher Site  Google Scholar
 N. Vukovic, N. Healy, and A. C. Peacock, “Guiding properties of large mode area silicon microstructured fibers: a route to effective single mode operation,” Journal of the Optical Society of America B: Optical Physics, vol. 28, no. 6, pp. 1529–1533, 2011. View at: Publisher Site  Google Scholar
 N. Healy, J. R. Sparks, R. R. He, P. J. A. Sazio, J. V. Badding, and A. C. Peacock, “High index contrast semiconductor ARROW and hybrid ARROW fibers,” Optics Express, vol. 19, no. 11, pp. 10979–10985, 2011. View at: Publisher Site  Google Scholar
 Y. Miao, B. Liu, K. Zhang, Y. Liu, and H. Zhang, “Temperature tunability of photonic crystal fiber filled with Fe_{3}O_{4} nanoparticle fluid,” Applied Physics Letters, vol. 98, no. 2, pp. 021103–021105, 2011. View at: Publisher Site  Google Scholar
 M.Y. Zhang, S.G. Li, Y.Y. Yao, B. Fu, and L. Zhang, “A dark hollow beam from a selectively liquidfilled photonic crystal fibre,” Chinese Physics B, vol. 19, no. 4, pp. 047103–047106, 2010. View at: Publisher Site  Google Scholar
 W. Qian, C.L. Zhao, J. Kang, X. Dong, Z. Zhang, and S. Jin, “A proposal of a novel polarizer based on a partial liquidfilled hollowcore photonic bandgap fiber,” Optics Communications, vol. 284, no. 19, pp. 4800–4804, 2011. View at: Publisher Site  Google Scholar
 G. P. Agrawal, Nonlinear Fiber Optics, Optics and Photonics Series, Academic Press, San Diego, Calif, USA, 4th edition, 2007.
 Q. Lin and G. P. Agrawal, “Raman response function for silica fibers,” Optics Letters, vol. 31, no. 21, pp. 3086–3088, 2006. View at: Publisher Site  Google Scholar
 http://www.cargille.com/.
 http://www.ufe.cz/costp11/.
 D. Jackson, “Towards highpower midinfrared emission from a fibre laser,” Nature Photonics, vol. 6, pp. 423–431, 2012. View at: Google Scholar
 B. T. Kuhlmey, B. J. Eggleton, and D. K. C. Wu, “Fluidfilled solidcore photonic bandgap fibers,” The Journal of Lightwave Technology, vol. 27, pp. 1617–1630, 2009. View at: Google Scholar
Copyright
Copyright © 2014 Partha Sona Maji and Partha Roy Chaudhuri. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.